Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Rectiverter wikipedia, lookup

Ohm's law wikipedia, lookup

Opto-isolator wikipedia, lookup

Resistive opto-isolator wikipedia, lookup

Power MOSFET wikipedia, lookup

Superconductivity wikipedia, lookup

Thermal runaway wikipedia, lookup

Lumped element model wikipedia, lookup

Transcript
```Band Structure and Electrical Conductivity in
Semiconductors
Amrozia Shaheen, Wasif Zia,
Asma Khalid and Muhammad Sabieh Anwar
LUMS School of Science and Engineering
Tuesday, September, 13, 2011
Semiconductors are one of the technologically most important class of materials.
According to the band theory of solids, which is an outcome of quantum mechanics,
semiconductors possess a band gap, i.e., there is a range of forbidden energy values
for the electrons and holes. In this experiment, we will calculate the energy band
gap in the intrinsic region and the temperature dependence of the majority carrier
mobility in the extrinsic region.
KEYWORDS
Semiconductor · intrinsic conduction · extrinsic conduction · energy band gap ·
conduction band · valence band · conductivity · resistivity · mobility · unijunction
transistor · temperature control · low temperature physics
Approximate Performance Time 2 weeks.
1
Objectives
In this experiment, we will,
1. understand how conductivity in semiconductors depends on carrier concentration and mobility, and how these depend on temperature,
2. distinguish between intrinsic and extrinsic temperature regimes and identify
the applicable temperature range from an examination of measured data,
3. appreciate and utilize the advantages of the four-probe resistance measurement technique,
4. calculate the energy band gap for doped Si and pure Ge,
1
5. calculate the temperature dependent coeﬃcient α of the majority carriers,
6. through experimental realizations, appreciate a physical understanding of
the band gap structure of semiconductors.
References
[1] C. Kittel, “Introduction to Solid State Physics”, John Wiley and Sons, (2005),
pp. 216-226.
[2] S. O. Kasap, “Principles of Electronic Materials and Devices”, Boston,
McGraw-Hill, (2006), pp. 378-405, 114-122.
[3] B. S. Mitchell, “An Introduction to Materials Engineering and Science”, New
Jersey, John Wiley and Sons, Hoboken, (2004), pp. 550-557.
[4] S. M. Sze, “Semiconductor Devices”, John wiley and Sons, (2002), pp. 41.
[5] J. Chan, “Four-Point Probe Manual ”, EECS 143 Microfabrication Technology, (1994), http://www.inst.eecs.berkeley.edu.
[6] “Low Level Measurements
http://www.keithley.com.
Handbook ”,
pp.
16-19/3,
50-51/4,
[7] A. Sconza and G. Torzo, “An undergratuduate laboratory experiment for measuring the energy gap in semiconductors”, Eur. J. Phys. 10 (1989).
[8] “CN1500
Series
Multi-Zone
http://www.omega.com.
Ramp
and
Soak
Controller ”,
[9] “Discrete PID controller ”, http://www.atmel.com.
2
2.1
Theoretical introduction
Semiconductors
The available energies for electrons help us to diﬀerentiate between insulators,
conductors and semiconductors. In free atoms, discrete energy levels are present,
but in solid materials (such as insulators, semiconductors and conductors) the
available energy states are so close to one another that they form bands. The
band gap is an energy range where no electronic states are present. In insulators,
the valence band is separated from the conduction band by a large gap while in
good conductors such as metals the valence band overlaps the conduction band.
Semiconductors have a small band gap between the valence and conduction bands
that allows thermal excitation of electrons from the valence to conduction band.
The overall picture is shown in Figure (1).
2
Electron Energy
Conduction
band
Band gap
Eg
E
f
Valence
band
Insulator
Conduction
band
Eg
E
f
Valence
band
Semiconductor
E
f
Conduction
band
Overlap
Valence band region
Metal
Figure 1: Simpliﬁed diagram of the electronic band structure of insulators, semiconductors and metals. The position of the Fermi level is when the sample is at
absolute zero temperature (0 K).
The Fermi level is an important consequence of band theory, the highest occupied
quantum state of electrons at absolute zero temperature. The position of the Fermi
level relative to the conduction band is an important parameter that contributes
to determine the electrical properties of a particular material. The position of the
Fermi level position is also indicated in Figure (1).
For a semiconductor, the electrical resistivity lies between a conductor and an
insulator, i.e., in the range of 103 Siemens/cm to 10−8 S/cm. An externally applied
electrical ﬁeld may change the semiconductor’s resistivity. In conductors, current
is carried by electrons, whereas in semiconductors, current is carried by the ﬂow
of electrons or positively charged holes.
Q 1. Explain (or sketch) the temperature dependence of resistance for metals
and semiconductors. Why does the resistance of a semiconductor decrease with
increasing temperature?
2.2
Intrinsic and extrinsic semiconductors
An intrinsic semiconductor is a pure semiconductor having no impurities. In an
intrinsic semiconductor, the numbers of excited electrons and holes are equal, i.e.,
n = p as shown in Figure (2a). An extrinsic semiconductor on the other hand is
the one in which doping has been introduced, thus changing the relative number
and type of free charge carriers.
An extrinsic semiconductor, in which conduction electrons are the majority carriers
is called an n-type semiconductor and its band diagram is illustrated in Figure (2b)
and the one in which the holes are the majority charge carriers is called a p-type
semiconductor and is indicated in Figure (2c). In extrinsic semiconductors, the
dopant concentration Nd is much larger than the thermally generated electronhole pairs ni and is temperature independent at room temperature.
Q 2.
Why is doping introduced in semiconductors? How does it eﬀect the
3
Conduction band
Ec
Ef i
E
c
Ef n
Ev
Ev
E
c
Ep
f
Ev
Valence band
(a)
(c)
(b)
Figure 2: Energy band diagrams for (a) intrinsic, (b) n-type, and (c) p-type semiconductors. Ef is the Fermi energy level, and the letters i, n, p indicate intrinsic,
n and p-type materials. Ec and Ev are the edges of the conduction and valence
bands.
conductivity of a semiconductor?
2.3
The ubiquitous role of semiconductor devices
Semiconductor devices are the foundation of the electronic industry. Most of these
devices can be constructed from a set of building blocks. The ﬁrst building block
is the metal-semiconductor interface as shown in Figure (3a). This interface can
be used as a rectifying contact, i.e., the device allows current in one direction as in
ohmic contact. By using the rectifying contact as a gate, we can form a MESFET
(metal-semiconductor ﬁeld-eﬀect transistor), an important microwave device.
Metal
n-type
p-type
semiconductor semiconductor
Semiconductor
(b)
(a)
Oxide
Semiconductor Semiconductor
a
b
Metal
Semiconductor
(d)
(c)
Figure 3: Basic device building blocks of (a) metal-semiconductor interface, (b) p-n
junction, (c) heterojunction interface, (d) metal-oxide-semiconductor structure.
The second building block is the p-n junction, a junction of p-type and n-type
materials indicated in Figure (3b). The p-n junction is the key compound for
numerous semiconductor devices. By combining two p-n junctions, we can form
the p-n-p bipolar transistor, and combining three p-n junctions to form a p-n-p-n
structure, a switching device called a thyristor can be formed.
4
The third important building block is the heterojunction interface depicted in Figure (3c). It is formed between two dissimilar semiconductors, for example gallium
arsenide (GaAs) and aluminium arsenide (AlAs) and is used in band gap engineering. Band gap engineering is a useful technique to design new semiconductor
devices and materials. Heterojunctions and molecular beam epitaxy (MBE) are
the most important techniques in which required band diagrams are devised by
continuous band-gap variations. A new generation of devices, ranging from solidstate photomultipliers to resonant tunneling transistors and spin polarized electron
sources, is the result of this technique.
The fourth building block is the metal-oxide-semiconductor (MOS) structure. It is
a combination of a metal-oxide and an oxide-semiconductor interface indicated as
in Figure (3d). The MOS structure is used as a gate and the two semiconductormetal oxide junctions are the source and drain; the result is the MOSFET (MOS
ﬁeld-eﬀect transistor). The MOSFET is the most important component of modern
integrated circuits, enabling the integration of millions of devices per chip.
2.4
Conduction in intrinsic semiconductors
The process in which thermally or optically excited electrons contribute to the
conduction is called intrinsic semiconduction. In the absence of photonic excitation, intrinsic semiconduction takes place at temperatures above 0 K as suﬃcient
thermal agitation is required to transfer electrons from the valence band to the
conduction band [3].
The total electrical conductivity is the sum of the conductivities of the valence and
conduction band carriers, which are holes and electrons, respectively. It can be
expressed as
σ = ne qe µe + nh qh µh ,
(1)
where ne , qe , and µe are the electron’s concentration, charge and mobility, and nh ,
qh , and µh are the hole’s concentration, charge and mobility, respectively.
The mobility is a quantity that directly relates the drift velocity υd of electrons to
the applied electric ﬁeld E across the material, i.e.,
υd = µE.
(2)
In the intrinsic region the number of electrons is equal to the number of holes, so
Equation (1) implies that,
σ = ne qe (µe + µh ).
(3)
The electron density (electrons/volume) in the conduction band is obtained by
integrating g(E)f (E)dE (density of states×probability of occupancy of states)
from the bottom to top of the conduction band,
∫ ∞
(4)
ne =
g(E)f (E)dE.
Ec
5
E
Conduction
band
E
E
E
Ec
Ef
Ec
Ef
E
v
E
v
Valence
band
0
g(E)
(a)
(b)
ne = ni
0.5
f(E)
(c)
n v = ni
1.0
ne (E) and n (E)
h
(d)
Figure 4: Band gap structure of an intrinsic semiconductor. (a) Schematic band
diagram, (b) density of states g(E), (c) Fermi distribution function f (E), (d)
carrier concentration ne (E) and nh (E). Ec , Ev and Ef represent the conduction
band energy, valence band energy and Fermi energy level, respectively.
There are two important quantities introduced in the above expression: g(E) is the
number of states per unit energy per unit volume known as the density of sates.
The density of states in the conduction band can be derived from ﬁrst principle
and is given by,
√
)1/2
3/2 (
( 2)m∗e
g(E) =
E − Ec
.
π 2 ~3
(5)
The function f (E) is the probability of an electronic state of energy E being
occupied by an electron, and is given by the Fermi-Dirac distribution function,
f (E) =
1
(
).
(E−Ef )
1 + exp kB T
(6)
The proﬁles of g(E) and f (E) are depicted in Figure (4). If we suppose that
E − Ef ≫ kB T , then Equation (6) can be approximated as,
(
)
E − Ef
f (E) ≈ exp −
.
kB T
(7)
Thus, we can replace the Fermi-Dirac distribution by the Boltzmann distribution
under the assumption that the number of electrons in the conduction band is far
less than the number of available states in this band (E − Ef is large as compared
to kB T ).
6
The number of mobile charge carriers (i.e., ne in the conduction band and nh in
the valence band) can be obtained by performing the integration in Equation (4),
and is given by,
)
(
−(Ec − Ef )
ne = Nc exp
,
(8)
kB T
and
nh
(
)
−(Ef − Ev )
,
= Nv exp
kB T
(9)
( ∗
)3/2
m e kB T
= 2
,
2π~2
(10)
( ∗
)3/2
m h kB T
= 2
.
2π~2
(11)
where
Nc
Nv
Nc and Nv are the eﬀective density of states for the edges of conduction and valence
bands, respectively [1].
Q 3. Derive the expressions (10) and (11) for the eﬀective density of states for
the conduction band, Nc , and for the valence band, Nv .
The terms m∗e and m∗h are the eﬀective masses of electrons and holes respectively, kB
is Boltzmann’s constant, T is the absolute temperature, and h is Plank’s constant.
Q 4. What do you understand by the term ‘eﬀective mass’ of an electron? How
is it diﬀerent from the conventional electron mass?
In an intrinsic semiconductor, the number of electrons is equal to the number of
holes, so the charge carrier concentration is given by,
ni =
√
(
ne nh =
)1/2
Nc Nv
)
−Eg
exp
,
2kB T
(
(12)
where, Eg = Ec − Ev is the energy band gap. The term (Nc Nv )1/2 in Equation (12)
depends on the band structure of the semiconductor. It will be shown later that for
intrinsic behavior, ni varies as some power of T , so Equation (12) can be written
as,
(
)
−Eg
3/2
(13)
ni = CT exp
,
2kB T
where, C is some constant. Substituting the expression (13) into (3) yield the
following expression for the intrinsic conductivity,
(
)
(
)
−Eg
3/2
(14)
σ = CT qe µe + µh exp
.
2kB T
7
Equation (14) shows that the electrical conductivity of intrinsic semiconductors
decreases exponentially with increasing temperature.
Q 5.
Derive Equation (12).
Q 6. Using Equation (14), explain how the conductivity of a semiconductor
changes at high temperatures.
Q 7. What is the diﬀerence between Fermi-Dirac and Boltzmann distributions?
Which distribution is being followed by the majority carriers in semiconductors?
Q 8. Given that the eﬀective masses of electrons and holes in Si are approximately 1.08 me and 0.60 me , respectively, and the electron and hole drift mobilities
at room temperature are 1350 and 450 cm2 V−1 s−1 , respectively, and the energy
band gap value is 1.10 eV, calculate the intrinsic concentration and intrinsic resistivity of Si [2].
2.5
Conduction in extrinsic semiconductors
In doped semiconductors, the dopant concentrations (ne ≃ Nd for n-type and
nh ≃ Na for p-type doping) at room temperatures are greater than the the thermally generated intrinsic carrier concentrations ni . The conductivity depends on
the carrier concentrations and the mobility. So to determine the temperature dependent conductivities, one has to consider, separately, how temperature aﬀects
both the carrier concentration and the mobility [2].
2.5.1
Temperature dependence of charge carrier concentration
Consider an n-type semiconductor with dopant carrier concentration (Nd ) of arsenic atom (As). The As atoms introduce a donor energy level Ed , that is located
at a gap ∆E below Ec . The ionization of As atoms leads to electrons jumping
across ∆E into the conduction band. The scenario is depicted in Figure (5).
1. Low temperature regime At very low temperatures, conductivity is almost zero because donor atoms are not ionized due to the small thermal
vibrational energy. As temperature slightly increases, the donor atoms get
ionized and move to the conduction band as shown in Figure (5a). The
electron concentration at such low temperature is given by,
(
)1/2
(
)
∆E
1
exp −
Nc Nd
(15)
ne =
,
2
2kB T
where, ∆E = Ec − Ed is the energy diﬀerence from donor energy level to
bottom of conduction band. The low temperature regime is also called the
ionization regime.
Q 9. What are the similarities and diﬀerences between Equations (12)
and (15)?
8
Conduction
band
Eg
Ef
Ed
+
As
As
As
As
Ef
As+
As+
As + As+
As+
As+
As+ As+
Ef
Valence
band
(a)
(b)
(c)
Figure 5: Electron concentration of an n-type semiconductor in (a) low temperature regime, (b) medium temperature regime, (c) high temperature regime. Ef
and Ed are the Fermi and donor atom energy levels, respectively.
log(n)
slope=-Eg /2kB
slope=-∆E/2kB
Intrinsic
region
Extrinsic
region
Ionization
region
1/T
Figure 6: The temperature dependence of the electron concentration in an n-type
semiconductor, showing the ionization, extrinsic and intrinsic regimes. Note that
the horizontal axis is 1/T instead of T .
Q 10. Explore the origin of the extra factor of one half in Equation (15).
2. Medium temperature regime In this temperature range, the process
of ionization has continued to the extreme that all donor atoms have been
ionized as shown in Figure (5b). This temperature range is often called
the extrinsic range and is also indicated in Figure (6). Since the electrical
conductivity depends on carrier concentration n and mobility µ,
σ = qnµ,
(16)
and n = Nd ≃constant in the extrinsic region, the conductivity is solely
determined by the temperature variation of the mobility. The mobility is
proportional to some power α of the temperature,
σ = T α.
9
(17)
A plot of log( σ1 ) versus log( T1 ) will give the value of temperature dependent
coeﬃcient α. Extrinsic semiconductors are almost always operated in this
region.
3. High temperature regime As temperature increases, the electron concentration ni due to thermal agitations across the band gap is much larger
than the dopant concentrations Nd . In this regime, excitations from valence
band to conduction band are also possible due to which hole concentration
becomes equal to the electron concentration nh = ne depicted in Figure (5c).
This range is referred as the intrinsic range and is shown in Figure (6). This
is the regime where the purpose of doping is defeated and the material behaves as an intrinsic semiconductor. In this temperature range, the slope of
log(n) versus 1/T yields (−Eg /2kB ).
Q 11. A silicon ignot is doped with 1016 As atoms/cm3 . Find the carrier
concentrations and the Fermi level at room temperature (300 K). Also draw band
diagram showing the Fermi level Ef and intrinsic Fermi level Ei [4].
Q 12. An n-type Si sample has been doped with 1015 phosphorus atoms cm−3 .
The donor level for P in Si is 0.045 eV below the conduction band edge energy [2].
(a) What would be the temperature above which the sample behaves intrinsically?
(b) What is the lowest temperature above which most of the donors are ionized?
2.5.2
Temperature and impurity dependence of drift mobility
Now that we have established how temperature aﬀects carrier concentration, we
turn attention to the mobility. Drift mobility µ determines the average velocity
υd in the presence of an applied external ﬁeld. The variation with temperature
follows two distinct regions.
1. High temperature region Let suppose an electron in the conduction (CB )
or valence band (VB ) suﬀers collisions from a scattering ion (As+ ). These
scattering events depend on how strongly the ions vibrate, the amplitude
depends on the temperature T . The mean free time τ between scattering
events, is given by,
τ =
1
Svth Ns
.
(18)
According to the Drude model [2], the drift mobility is,
µ =
eτ
.
m∗e
(19)
In Equation (18), S is the cross-sectional area of the scatterer shown in Figure (7a), vth is the mean speed of the electrons, called the thermal velocity
and Ns is the number of scatterers per unit volume. Now both the scatterer
10
νth
amplitude
t=t1
Effective scattering
cross-section
t=0
Scatterer mean
position
S=πa 2
a
t=t2
(a)
(b)
Figure 7: (a) Scattering cross-section, (b) scatterer position at three diﬀerent times
t = 0, t = t1, t = t2.
amplitude a and the thermal velocity of the electron vth is temperature dependent. We unveil these dependences, one by one. The scatterer amplitude
increases with temperature as a2 ∝ T . Now an electron in the conduction
band has only kinetic energy and the mean kinetic energy per electron in the
conduction band is 23 kB T . Applying kinetic molecular theory to the gas of
electrons in the conduction band, we obtain,
1 ∗ 2
3
me vth =
kB T,
2
2
(20)
implying vth ∝ T 1/2 . Using the above derived temperature dependences of
vth , the scatterer mean time τL due to lattice vibrations will become,
τL =
1
1
∝ 3/2 = T −3/2 ,
Svth
T
(21)
resulting in lattice vibration scattering limited mobility, µL ,
µL ∝ T −3/2 .
(22)
Clearly as the temperature goes up, µL decreases.
2. Low temperature region At low temperatures, the scattering of electrons
by thermal lattice vibrations is not strong enough. The electron scattering is
performed by the electrostatic interaction with the ionized donor impurities.
Let us consider a case in which an electron passes by an ionized donor As+ .
The deﬂection from the rectilinear path depends on the following factors,
• If the K.E of the electron is larger than the P.E of the ionized donor
impurity (As+ ) at a distance r (K.E > |P.E|), then the electron will
not feel the P.E and will continue its course unhindered, unswayed.
11
e-
K.E>IP.EI
K.E=(1/2)mev 2
K.E~IP.EI
∼
rc
As+
K.E<IP.EI
Figure 8: Electron scattering by an ionized impurity (As+ ) that is ﬁxed in position.
• If the K.E < |P.E|, then the columbic interaction energy is strong
enough to deﬂect the electron. The two cases are depicted in Figure (8).
• K.E ≈ |P.E| at r = rc , the critical radius at which the electron is just
3
e2
kB T =
,
2
4πεo εr rc2
(23)
from which one can deuce the critical radius,
log(µ)
rc =
T
e2
.
6πεo εr kT
(24)
T -3/2
3/2
Impurity Scattering
Lattice Scattering
log(T)
Figure 9: Temperature dependence of mobility including eﬀects of both lattice and
impurity scattering in the two temperature regimes.
Thus, the critical scattering radius rc also possesses the inverse temperature dependence and decreases as temperature increases. By adding
the value of rc into scattering cross section, S = πrc2 , one may infer that
12
S ∝ T −2 . Therefore, the ionized impurity scattering limited mobility,
µI comes out as replacing the same argument given before Equation (22)
µI ∝
T 3/2
,
NI
(25)
where NI is the ionized impurity concentration. Thus in the low temperature regime, µI decreases with increasing ionized impurity concentration.
The lattice limited and impurity limited regimes of the mobility are shown in Figure (9). It is observed from Equations (22), (25) and Figure (9) that the mobility
has a divergent behavior with respect to temperature. At low temperature, mobility increases with increasing temperature, and starts decreasing as temperature
increases in the high temperature regime.
Q 13. Calculate the temperature dependence of the mean free time τ between
impurities and derive Equation (25).
2.6
Temperature dependence of conductivity
We have determined the temperature dependence of the carrier concentration and
mobility for a doped semiconductor. Hence, the electrical conductivity in extrinsic
semiconductors can be determined by combining the results of Figures (6) and (9),
as shown in Figure (10).
log(n)
slope=-Eg /2kB
Extrinsic
region
log µ
log(n)
slope=-∆E/2kB
T -3/2
Intrinsic T 3/2
region
log(µ)
Ionization
region
1/T
Figure 10: Combined eﬀects of mobility and carrier concentration.
13
3
The experiment
3.1
Overview of the experiment
In this experiment we will investigate the conductivity temperature variation of a
semiconductor sample (the base region in the unijunction transistor UJT(2N2646)
and pure germanium Ge). The conductivity is derived from the measured resistance while temperature is controlled by a controller and measured using a
thermocouple.
The semiconductor sample is placed inside a sample cell. The sample cell is placed
inside a ﬂow cryostat which can be ﬁlled by liquid nitrogen. The cell is cooled by
the cool vapor of N2 . Alternatively, the cell can be heated to elevated temperatures
by passing current through a heater wire wound around it. The ﬂow cryostat is
sketched in Figure (11a) highlighting the various components.
The resistance of the semiconductor sample is measured by the four-probe technique [5], [6]. A constant current is passed through the sample. The current is
generated by a constant current source. The voltage drop across the sample is
acquired by a four-probe circuit and facilitated by a Labview programme. To
measure the temperature of the sample, a K-type thermocouple is placed inside
the sample cell and the temperature control is achieved by a multi-zone controller.
The measured resistance at diﬀerent temperatures yields the conductivity versus
temperature behaviour of the semiconductor sample, from which the energy band
gap Eg and the temperature dependent coeﬃcient of mobility α can be calculated.
3.2
Apparatus
The experiment involves the following major components.
1. cryostat
2. sample cell containing the sample and wound with heater wire
3. temperature controller
4. thermocouple
5. voltmeter with high input resistance
6. constant current source
7. power supply for the constant current source
8. solid state relay (SSR)
9. data acquisition system (DAQ)
14
Sample cell
Thermocouple
Variac
I
V
Funnel
100V
Pipe
+ Output
- Channel +Input
+5V
Input Output
-5V
Solid state
relay (SSR)
Channel
L1
L2 Power
Temperature
controller
Insulating lids
Thermocouple
(b)
Cryostat
Sample cell
Sample
Liquid nitrogen
Heat sink
Stand
(a)
(c)
Figure 11: Experimental setup: (a) cryostat with the sample cell, (b) circuitry of
the temperature control setup, and (c) assembled view. I is the input constant
current and V is the measured voltage.
10. supply of liquid nitrogen N2 .
Following some brief description of the above listed components.
3.2.1
Samples
The samples used for band gap measurements are pure Ge (donated by Dr. S. A.
Siddiqi (Punjab University) and extremely expensive!)and the base of a unijunction
transistor UJT (a lightly doped n-type material).
Pure Ge was powdered and pressed in to a pellet of diameter d = 1.3 cm and
thickness t = 0.65 cm. When used in Four probe technique, the distance between
voltage wires was kept s = 0.25 cm. The sample was treated as a bulk material
since the sample thickness is signiﬁcantly larger than the spacing between voltage
wires. The resistivity is measured from the following expression [5],
V
ρ = 2πs ,
I
(26)
where I is the current applied to the sample from the constant current source and
V is the voltage drop across the sample.
15
3.2.2
Cryostat
The cryostat, shown in Figure (12a) is a copper cylinder (4 inch in diameter,
12 inch long with one end closed), used to maintain cryogenic temperatures, and
also able to withstand high temperatures. An insulating sheet is wrapped around
the cylinder for reducing heat losses.
(a)
(b)
Figure 12: (a) Cryostat. (b) Sample cell with heat sink.
3.2.3
Sample cell
For high temperature measurements, the semiconductor sample is slowly heated
inside the sample cell wound with nichrome heater wire (Nichrom 37). It is essentially a copper pipe (20 mm diameter with one end closed). For low temperature
measurement, a copper braid is attached to the bottom of the sample cell that
serves as a heat sink, and is shown in Figure (12b). The heat sink ensures good
thermal contact with liquid nitrogen. The sample cell is lowered into the cryostat
for the measurements.
3.2.4
Thermocouple
A thermocouple is a temperature sensor used to measure the sample temperature.
It is made up of two diﬀerent metals with the metals at one end joined together.
Whenever the junction of two metals is heated or cooled, voltage is produced
that can be correlated with temperature through a calibration procedure. In this
experiment, we use a K-type thermocouple, for which some details are given in
Table (1). The thermocouple reading is fed into a multi-zone controller.
16
temperature range
composition
sensitivity
−200 o C to 1250 o C
Chromium-Aluminium
∼ 41 µV/o C
Table 1: Some characteristics of the K-type thermocouple.
3.2.5
Temperature controller
Our aim is to attain a stable temperature for the sample, for which a multi-zone
controller (CN1504-TC from Omega Engineering) is used. It is a compact unit
comprising four PID controllers, and is shown in Figure (13). Additionally, it is
also equipped with an ON/OFF control [8]. A temperature proﬁle is programmed
into the controller to achieve a particular temperature for a certain duration of
time. To obtain an understanding of the programming modes and a guide to
constructing the proﬁles, refer to Appendix A or the datasheet of the controller
[8].
(a)
(b)
Figure 13: Temperature controller, (a) front view, (b) rear view.
The advantage of the temperature controller is that it posseses a “Proportional,
Integrator, Derivative” (PID) controller. The PID controller calculates an error
value as the diﬀerence between a measured process variable and a desired set point.
For more details see Appendix B.
Q 14. Read Appendix A. Programme a proﬁle in the temperature controller.
Your starting point will be the room temperature, achieve 40◦ C in 1 min and keep
the temperature ﬁxed at 40◦ C for 10 minutes. Subsequently, migrate to 50◦ C in
1 min and keep the temperature ﬁxed at 50◦ C for 10 minutes.
The purpose of the previous step is to familiarize you with the programming of the
temperature controller. This step must be completed and practised before
the start of the experiment.
17
3.2.6
Four-probe versus two-probe method
Resistance measurements are often taken by a two-probe method, that is depicted
in the self-explanatory Figure (14a). The disadvantage of this method is that
some voltage drop occurs across the lead resistance, hence the voltage measured
by the meter (Vm ) will be diﬀerent from the actual voltage (Vr ) across the test
resistance. So when applied to low test resistances (Rx < 100 Ω), the voltage
drop due to current (Ilead ) ﬂowing through the lead resistance can no longer be
neglected, leading to signiﬁcant error in the results.
In order to remove the error of contact resistances, a four-probe method is preferred, specially when Rx is small. In this method, current is passed through the
test resistance using one set of leads and voltage drop is measured through another
set, as depicted in Figure (14b). Although small current may ﬂow through the voltage measuring leads but that would be much smaller, owing to the extremely large
input resistance of the voltmeter, and can generally be neglected for all practical
purposes [6].
3.2.7
Constant current source and voltmeter
The resistance of the semiconductor sample is measured by passing constant current through the sample and measuring the voltage drop generated across it. In
order to provide stable current to the sample, a constant current generator is required and is shown in Figure (14c). You are required to construct this
constant current source. The sample resistance (Rx ) is calculated from the
output voltage as,
Rx =
Vo
I
= R(
(27)
Vo
),
Vz
(28)
where Vz is the Zener voltage and Vo is the output voltage that will ultimately
Semiconductor sample
Unijunction transistor (UJT)
Germanium (Ge)
Rx
up to 10 kΩ
<1 kΩ
I
100 µA
10 mA
Table 2: Current (I) required for semiconductor samples.
provide the sample resistance given in Table (2). Figure (14c) shows a circuit that
generates 1 mA current. The operational parameters for the various samples that
will be used in this experiment are given in Table (2).
The overall four-probe circuit including a current source and a voltmeter, based on
a diﬀerential ampliﬁer [10], is drawn in Figure (14d). Two separate contact pairs
are made on both ends, (AB) for passing current and (CD) for voltage detection,
as indicated in Figure (14d). The output from the voltmeter is fed into the data
acquisition system (DAQ).
18
I
Vm
R
Vm
RX
Vr
Vm
I
Rx
Vr
Vm =Votage measured by meter
Vr =Voltage across resistor
Measured resistance=
Measured resistance= Vm = R+(2* Rlead )
I
(a)
Vm
I
=
Vr
I
(b)
-12V
rc
680Ω
12V
2.7kΩ
5kΩ
Vz
2.7V
A
-12V
50KΩ
680Ω
2.7KΩ
+
1/4TL084
2.7V
rc
-12V
(c)
+
C
I
1/4TL084
1KΩ
1KΩ
+
1/4TL084
Rx
B
RX
TL081
+
-1/4TL084
+
D
1KΩ
Vo
1kΩ
(d)
+18V
220V
AC
D1
D2
LM317
+ve
D4
-18V
D3
+
- C2=10µF
+
C1=1000µF
-
+12V
110Ω
+
- C5=10µF
1 kΩ
GND
+
-
+ C4=10µF
-
C3=1000µF
(e)
-ve
LM337
1kΩ
110Ω
+ C6=10µF
-12V
Figure 14: The Electronic circuitry. (a) 2-probe method, (b) 4-probe method,
(c) current source, (d) overall circuit showing the current source and diﬀerential
ampliﬁer, (e) DC power supply.
Q 15. Make circuits capable of providing stable currents of 100 µA and 10 mA.
Q 16.
(14d)?
What is the gain of the diﬀerential ampliﬁer circuit given in Figure
19
Q 17. What is the advantage of a diﬀerential ampliﬁer as compared to an
ordinary ampliﬁer.
3.2.8
Power supply
In order to supply DC voltage to the constant current source and voltmeter, a
bipolar power supply is used in which AC voltage is converted to a selectable DC
voltage. The home built power supply is already provided to you. For interested
students, the circuit description of the supply is presented in Figure (14e). The
(b)
(a)
Figure 15: (a) open view, (b) closed view.
assembled circuit is photographed in Figure (15a) and enclosed in an aluminium
box depicted in Figure (15b). The BNC connectors provide +12 V, −12 V and
ground points.
3.3
Experimental procedure
1. Make circuits for constant current sources of 100 µA, 10 mA and the voltmeter on bread board according to the circuit diagrams in Figures (14c),
(14d).
2. You are provided with one unijunction transistor (UJT) and a pellet of pure
germanium (Ge). Current and voltage wires have already been connected
using silver paint with these samples, shown in Figure (16).
3. Pass the insulated wires, enshrouded in a ceramic rod through the steel
pipe. Connect current and voltage leads with constant current source and
voltmeter. You will acquire voltage through the data acquisition system
(DAQ).
4. Before making any electrical connection, set the output voltage of the variac
to 100 V. Measure it with a voltmeter.
5. Layout the experiment as suggested in Figure (11). Do not switch on power
at this satge.
6. Connect the solid state relay (SSR) with the sample cell as well as with
the temperature controller, in a way that its positive terminal is connected
20
current and
current and
ceramic rod
(a)
(b)
Figure 16: (a) Pure germanium Ge. (b) Unijunction transistor UJT.
to the positive output channel of the temperature controller, and negative
terminal is connected with the negative output channel of the controller. The
remaining terminals are connected to the sample cell and variac, as sketched
in Figure (11b).
7. Open the Labview ﬁle titled energyband.vi. Make a folder, and enter your
ﬁle name (e.g D:\amrozia\test.lvm). Your data will automatically be saved
in that ﬁle. You will use the DAQ system together with the Labview code
to measure the output voltage of the four-probe circuit.
8. First set the variac at 100 V. Switch on the variac, the temperature controller
will turn on. Leave the setup for 10 minutes to warm up the temperature
controller.
9. Turn on the DC power supply that is connected to the current source and
voltmeter. Check the output of the voltmeter.
10. UJT sample, low temperature measurement:
• It is not required to programme the temperature controller in this phase
of the experiment as the temperature is naturally increasing.
• Add liquid nitrogen to the cryostat through the funnel.
• The temperature controller will start showing the corresponding temperature. Pour liquid N2 until you reach the temperature ∼ (−150◦ C).
• Leave the setup to warm up to room temperature. As it warms, do the
following.
• Take voltage measurement after every 10◦ C rise in temperature using
the Labview ﬁle energyband.vi.
• Suppose the temperature controller shows −150◦ C. In the front panel,
enter the value −150◦ C in the temperature box. Press the run button to
start acquiring data and the stop button to stop running the acquisition,
while the temperature is still −150◦ C.
21
• Open Matlab, and add the appropriate folder to the Matlab path.
• Take the mean of the voltage value at the diﬀerent temperatures.
11. UJT sample, high temperature measurement:
• When you have reached room temperature, you will start taking your
readings for higher temperatures. For this purpose, you will require the
heater and the PID controller.
• Suppose you want to take readings in steps of 10◦ C, ranging from 40◦ C,
50◦ C, up to 250◦ C.
• Suppose the room temperature is 32◦ C.At this point we need to enter
a proﬁle so that the temperature negotiates 40◦ C, 50◦ C and 60◦ C, as it
is only possible to programme for these three points at one time. Now
enter this temperature proﬁle according to the instructions in Appendix
A.
• Acquire the voltage for 40◦ C, 50◦ C and 60◦ C using Labview as discusses
earlier.
• For the next set of points (e.g 70◦ C, 80◦ C, 90◦ C), you will have to repeat
the above steps.
• Complete your measurements up to ∼ 250◦ C.
• Find resistance from the acquired voltage.
• Tabulate temperature versus resistance, as indicated in Table (3).
Temperature (◦ C)
−150
−140
.
.
250
Resistance (Ω)
Table 3: Relationship between temperature and sample resistance.
12. Ge sample, high temperature measurement:
• You are provided with a pure Ge sample, an intrinsic semiconductor.
Set up the complete experiment being guided by your experience with
the UJT sample. The constant current for the Ge sample is I = 10 mA.
• Again enter the temperature proﬁle in the temperature controller. You
will require measurements up to 150◦ C.
• Complete acquiring the data.
• Tabulate temperature versus resistance.
Q 18. Plot a graph of log( R1 ) versus T in Kelvins, and distinguish the intrinsic
and extrinsic regions for the UJT.
22
Q 19. Calculate the energy band gap from the intrinsic region data for UJT
and Ge. As conductivity depends on both the charge carrier concentration and
mobility, so in calculating band gap take both of these factors into account. The
published energy band gap values for silicon (Si) and germanium (Ge) are provided
in Table (4).
Semiconductor
Silicon (Si)
germanium (Ge)
Band gap
1.12 eV
0.67 eV
Table 4: Energy band gap (Eg ) for Si and Ge.
Q 20. Calculate the temperature coeﬃcient α of the carriers mobility from the
extrinsic region data of the UJT. The published value of α is 2.3, given in [10].
Q 21.
What is your uncertainty in the energy band gap measurement?
Q 22. In the low temperature measurements, the sample is continuously thawing (warming) as data is being acquired. What kind of uncertainty does this cause
A
How to construct a temperature profile in temperature controller
Temperature range (oC)
Suppose we want to make the temperature proﬁle, sketched in Figure (17). For
this you have to do the following steps.
Setpt#5
60
Setpt#3
50
Setpt#1
Setpt#4
Setpt#2
40
Setpt#6
10 min
1 min
10 min
1 min
10 min
1 min
32
0
Time
Figure 17: An example of temperature proﬁle. Setpt#1, 2 is 40◦ C, setpt#3, 4 is
50◦ C, and setpt#5, 6 is 60◦ C.
1. The very first and the most important step is to power up the
temperature controller. Power connections should be made to L1, L2.
23
L1 is connected to the positive terminal of the AC power supply and L2 with
the negative one. Our AC power supply is the variac, and it should be set at
100 V. Be careful in applying voltage to the temperature controller
as it can be damaged, if you operate it over 120 V AC.
2. To enter into the programming mode, hold the CTR.SEL key until the unit
displays EntEr PASSCOde. At this point, enter the pass code which is
3254 for our device.
3. Select programme system PrG SYS mode, the controller will enter into
the system conﬁguring mode. Push PROG key, the display will show dSP
OPt, select Process-Setpoint. You have to push PROG key to go to the
next mode. The display will show dSPLy t, enter time in seconds using NH
and < DIG > keys. The NH and < DIG > keys are used to assign values.
Select Strt SP mode. Assign a value of 10 to rAtE tb mode. Enter COLd
JN value that would be the room temperature. Enter a value of 10 to the
V rAnGE mode and next to it, assign value to the C RAnGE that would
be 20.
4. Move to the programme control PrG Ctr mode. Push PROG key, the
display shows CntrL x (where x=controller no.), select controller 1. Then
go to Ct tYPE mode and select PID option. Select Cr.Al (for the Ktype thermocouple) for SIGnAL mode. Then select dEGrE C and ﬁnally,
select engineering unit mode Cx UNIt that would be C if input signal is a
thermocouple.
5. Next select the tuning mode. Push PROG key until the unit displays tUnIng. Select the PID mode. Enter the following values as,
• proportional band = 0.5,
• reset = 1,
• rate = 1.
6. Push PROG key to enter into proﬁle mode. When the unit displays the
PROFILE, select the required controller (controller 1) using PROG key.
When the display will brieﬂy read Strt SP, enter the value of starting set
point that would be room temperature, for example 32◦ C as indicated in
Figure (proﬁle). Use NH and < DIG > keys to enter the desired value. Next
press SETUP to go to the next function. At this point the display will
brieﬂy read SetPt 1 enter the value of setpoint 1, for example 40◦ C. Push
PROG key to go on to the next step. The display will show EntEr t, enter
the time value like 1 min. Move to setpoints 2 by pressing PROG key. Enter
setpoint 2 value which is 40◦ C and time=10 min. Repeat the above steps to
program up to setpoint 6 as shown in Figure (17).
7. Push EXT key. Again push EXT key for saving programme. Select the
desired controller using PROG key and run it by pressing RUN/STOP
key.
24
B
PID controller
The PID controller manipulates the process inputs based on the history and rate
of change the signal [9]. The basic idea is that the controller reads the system by
a sensor as shown in Figure (18a). Then it subtracts the measurement from the
desired reference to generate the error value. The error will be managed in three
ways: to handle the present through the proportional term; recover from the past
using the integral term; and to anticipate the future through the derivative term.
setpoint
Σ
error
P
Kpe(t)
I
Ki e(t)
t
Σ
0
process
output
D Kd ddte(t)
sensor
(a)
response
setpoint overshoot
rise time
time(s)
(b)
Figure 18: (a) Block diagram of a PID controller. (b) Response of a PID closed
loop system.
B.1
Proportional term
The proportional term (sometimes called gain) changes the output in proportion to
the present error value. The proportional response can be adjusted by multiplying
the error by a constant KP called the proportional gain. A high proportional gain
results in a large change in the output. If the proportional gain is too high, the
system can become unstable. In contrast, a small gain results in a small output
response, and a less responsive controller.
25
B.2
Integral term
The integral term (sometimes called reset) is proportional to both the magnitude
and duration of the error. This term sums up the previous errors to the system
control input. The summing of the error will continue until the system process
value equals the desired value, and this results in no stationary error. The magnitude of the contribution of the integral term correction is determined by the
integral gain Ki .
B.3
Derivative term
The derivative term (also called the rate) calculates the rate of change of the
process error by determining the slope of the error over time. The magnitude of the
contribution of the derivative term to the overall system is determined by the term
Kd . The derivative term slows the rate of change of the controller output. However,
derivative control is used to reduce the magnitude of the overshoot produced by the
integral term and improve the controller-process stability. If the derivative term
is too large, it can cause the process to become unstable as this term is highly
sensitive to noise in the error.
26
```
Related documents